# Electrostrictive Mechanism of Nanostructure Formation at Solid Surfaces Irradiated by Femtosecond Laser Pulses

- Oleg R. Pavlyniuk
^{1}Email author and - Vitaly V. Datsyuk
^{1}

**11**:16

https://doi.org/10.1186/s11671-015-1224-5

© Pavlyniuk and Datsyuk. 2016

**Received: **27 November 2015

**Accepted: **28 December 2015

**Published: **12 January 2016

## Abstract

The significance of the mechanical pressure of light in creation of laser-induced periodic surface structures (LIPSSs) is investigated. Distributions of the electrically induced normal pressure and tangential stress at the illuminated solid surface, as well as the field of volume electrostrictive forces, are calculated taking into account surface plasmon polariton (SPP) excitation. Based on these calculations, we predict surface destruction and structure formation due to inelastic deformations during single femtosecond pulses. The calculated fields of the electromagnetic forces are found to agree well with the experimental ripple structures. We thus conclude that the electrostrictive forces can explain the origin of the periodic ripple structures.

## Keywords

## Background

Femtosecond laser-pulse interaction with matter can lead to formation of laser-induced periodic surface structures [1–3]. Various applications of the laser-induced periodic surface structures (LIPSSs) have been proposed. They can be used for building microfluidic channels, controlling over laser marking and changing the color of materials [4, 5], overcoming the diffraction limit in laser nanomachining [6], modifying local electrical properties, improving the efficiency of solar cells [7], grating production, and optical data storage [8].

Though LIPSS was first observed in 1965 [9], the origin of the ripple structures is still debated [10]. Two types of basic formation mechanisms explained the observed structures. The first was a resonant mechanism based on (i) periodic electromagnetic-energy deposition due to roughness of the surface [11] or (ii) excitation of surface plasmon polaritons (SPPs) [1, 2, 6, 12–14]. The second non-resonant mechanism was related with thermal consequences of laser irradiation of the target, for example, capillary waves formed in the melted layer [15].

The classical resonant model [11] of the LIPSS formation assumed scattering of the incident laser wave by surface roughness and interference of the laser beam with refracted light. This interference causes inhomogeneous electromagnetic energy absorption just beneath the surface. According to this model, the period of the energy deposition can be smaller than the laser wavelength. However, initial roughness at the surface and several laser pulses are required to form LIPSS in this case [6]. In [16], the finite-difference time-domain method was applied to study the inhomogeneous energy absorption of a linearly polarized laser beam below the rough surface. The numerical results confirmed the resonant scenario.

A resonant mechanism for ripple formation involved excitation of the surface electromagnetic wave by the incident laser irradiation [1, 2, 6, 11–18]. According to [1, 6, 12, 14, 15, 17, 18], interference of the laser light with SPP creates periodic field distribution at the interface, which in some way leads to growth of a structure with the same period.

The SPPs can be excited at a metal surface. Therefore, LIPSS-covered metals were explained by SPP excitation [13, 14]. In addition, LIPSSs were observed at surfaces of semiconductors [1, 2, 12, 15, 17] and dielectrics [2, 6, 12]. Therefore, the possibilities and conditions of SPP excitation in semiconductor and dielectric materials were studied in [1, 2, 6, 12, 15].

Among the non-resonant mechanisms, it can be mentioned a theoretical model comprising heat transfer and hydrodynamic components [15]. The heat transfer component described particle dynamics, carrier excitation, and heat conduction phenomena. The hydrodynamic component described the molten material dynamics and the process of capillary wave solidification.

It should be noted that the timescale of the femtosecond laser pulses and SPPs (≃fs) is significantly less than the expected timescale of material movement (≃ps) [18] in the processes described above. Moreover, some authors [1, 17, 18] have demonstrated the possibility of the LIPSS creation just with a single femtosecond pulse. All these facts allow us to assume that mechanical action of the electromagnetic field can play an important role in the ripple formation. Therefore, the goal of our study is to determine the electromagnetic forces exerted on the material surface allowing for interference of the incident electromagnetic field with the excited SPP. We define a distribution of the electrically induced normal pressure and tangential stress at metal surface and estimate their amplitudes. In addition, we evaluate a density of the volume forces inside the surface layer. Then, we check correspondence between our calculations and known characteristics of the ripple structures.

## Methods

We applied the classical electromagnetic theory both to determine the properties of the SPPs and to calculate the force acting on a metal surface. For simplicity, we consider the interaction of a femtosecond laser pulse with a nonmagnetic metal (*μ*
_{2}=1 at *z*>0) in air (*ε*
_{1}=1, *μ*
_{1}=1 at *z*<0).

### Surface Plasmon Polaritons

In most cases, the ripples were observed to be perpendicular to the electric field vector [1–3, 6, 11–14]. Therefore, their origin was attributed to SPPs excited by a TM polarized mode [1, 3, 6, 7, 12, 14, 15, 17, 18].

*k*

_{p}follows from the Maxwell’s boundary conditions giving

where *k*
_{0}=*ω*/*c* is the vacuum wave number, *c* the speed of light in vacuum, and *ε*
_{1} and *ε*
_{2} are the permittivities of the media at frequency *ω*.

According to Eq. 1 and conditions of SPP existence (one of dielectric constants is negative with an absolute value exceeding that of another) [19, 20], *k*
_{p} is always larger than *k*
_{0}. Therefore, the SPP can be excited if there are nanoparticles at the surface and a localized plasmon excited around it [20]. The required nanoparticles can be created by electromagnetic forces acting on nanobubbles under the surface of metal [22].

### Maxwell Stress

**n**is the external unit vector normal to the surface,

**T**the Maxwell stress tensor, and brackets denotes averaging over time. Among several forms of the Maxwell stress tensor, we chose one introduced by Lorentz

where *ε*
_{0},*μ*
_{0} are the permittivity and permeability of vacuum, ⊗ denotes the outer product, and **I** is the unit matrix. The Maxwell-Lorentz tensor takes into account electrostriction and agrees with experiments better than other stress tensors [24].

**T**with

**n**has a jump. The difference between 〈

**T**〉·

**n**in two media gives the surface force \(\pmb {{\mathcal {F}}}\) which is measured in pascals. In order to relate the

*z*-component of \(\pmb {{\mathcal {F}}}\) with the normal pressure

*P*on metal surface, we use the following definition:

where \(\hat {\mathbf {z}}\) is a unit vector in the direction of the *z*-axis; the tangential component of \(\pmb {\mathcal {F}}\) is called the tangential stress **S**. Formulas for calculating *P* and **S** are given in Appendix 2.

## Results and Discussion

**E**just beneath the surface (see Appendix 2). This field is a superposition of the transmitted electric field and the electric field of the surface plasmon wave

**E**

_{2}. The normal pressure is expressed through the square of the normal component of

**E**averaged over time. Here, we consider the incidence of a plane electromagnetic wave with the magnetic field parallel to the interface

*z*=0, i.e., the case of p-polarization. In this case, the normal component of the electric field is nonzero and

*E*

_{ n }=

*E*

_{ z }. We neglect the reflected wave and took into account that the frequency

*ω*of the incident wave is close to the plasmon frequency

*ω*

_{s}(usually, the central wavelength of the the femtosecond laser is at 800 nm). Under these assumptions, we obtain

*E*

_{iz }and

*k*

_{ix }are the

*z*-component of the electric field and the

*x*projection of the wavevector

**k**of the incident wave, respectively;

*E*

_{2z }is the

*z*-component of the SPP field defined by Eq. 19. Unlike the normal pressure, the tangential stress depends on both the tangential and normal components of the electric field. Therefore, we calculate

*θ*is the incident angle, then

*k*

_{ix }=

*k*

_{0}sin

*θ*and

*λ*

_{0}=2

*π*/

*k*

_{0}is the wavelength of the incident wave and

is the wavelength of the SPP.

where + corresponds to backward-propagating SPPs. The found periodicity is the same as the periodicity of the LIPSSs measured and estimated by a number of authors [6, 11, 12, 14, 15, 17, 18].

*P*and

*S*of Appendix 2 and Eqs. 7 and 8, we evaluated the magnitude of the surface force. All calculations were performed using the permittivity copper equal to

*ε*

_{2}=−25.07+2.54

*i*at a wavelength of 800 nm. According to [1, 6, 15, 17], the amplitude of the electric field of the SPP can be of the order of the electric field of the incident wave. We took

*E*

_{i}through the laser parameters

*Φ*is the fluence of the laser pulses and

*τ*is the pulse duration. Lasers with

*τ*=140−150 fs,

*λ*

_{0}=800 nm and

*Φ*in a range of 0.2−1.5 J/cm

^{2}are commonly used to generate LIPSSs. In numeric estimates, we used

*τ*=150 fs and

*Φ*=1 J/cm

^{2}giving

Textbooks in optics identify *P*
_{0} as the pressure of light on a perfectly absorbing medium with zero reflection coefficient [20]. If the reflection coefficient is equal to unity, the pressure would be equal to 2 *P*
_{0}. If *ε*
_{1}=1, light always pushes the absorbing medium exerting positive pressure, according to the common understanding of the radiation pressure. In this letter, we applied the Maxwell-Lorentz stress tensor to define the pressure *P* acting on a surface layer of a solid. In the case of normal incidence of light without plasmon excitation, one gets *P*=0 since *E*
_{
n
}=0. The normal component of the electric field is not zero if SPPs are generated. Using Eq. 12, we got *P*≃−12 *P*
_{0} and a periodic *S*
_{
t
} varying with a period *Λ*=*λ*
_{s}≃770 nm and amplitude 5 *P*
_{0} at the surface of copper.

**f**. Thus, we found a distribution of

**f**in copper for the case of normal incidence of a plane electromagnetic wave following by SPP excitation. The result of the calculation is presented in Fig. 2 which represents

**f**in units of \(f_{0}= \frac {1}{2}\, \epsilon _{0}\left |\mathbf {E}_{i}\right |^{2} \times 10^{9}\) m

^{−1}. The integral \(\int _{0}^{\infty } \mathbf {f}\,\mathrm {d}z\) gives as the pressure on a tin semi-infinite cylinder with the axis coincident with the

*z*axis. The value of this pressure was found to be 50

*P*

_{0}. The volume force is distributed in a surface layer with a depth of about 25 nm. Our calculation thus show that the magnitudes of the surface and volume pressures can be as large as a few gigapascals. Such pressures should result in inelastic deformation of copper according to [25]. Figure 2 implies that a depth of the grooves created by a single femtosecond pulse could be about 25 nm.

We also established the period of the volume forces in the *x* direction. It is equal to 770 nm that is less than *λ*
_{0}=800 nm. The former number coincides with the period *λ*
_{s} of the tangential stress found from Eq. 11 for the normally incident wave when *θ*=0.

## Conclusions

In this letter, we have proposed an electrostrictive mechanism of the LIPSS formation. We have calculated the electrically induced normal pressure and tangential stress exerted on the air-copper interface under interference of the incident laser field with the excited SPP. In addition, we determined the electrostrictive volume forces to a metal surface layer. The interfacial stress and the pressure on the surface layer have been found to reach a few gigapascals which is sufficient for copper surface modification. These calculations demonstrate that electromagnetic forces could be very important in the process of the LIPSS formation. The predicted period of the surface force distribution is in good agreement with the experimentally observed LIPSS periods and those given by other theoretical models. In the framework of the proposed theory, the depth of the grooves created with a single femtosecond laser shot has been also estimated.

## Appendices

### Appendix 1. Electric Field of Surface Plasmon Polariton

SPP is an electromagnetic excitation that may exist at the interface of two media with dielectric constants of opposite signs (for instance, dielectric and metal) [19, 20]. The electric and magnetic fields satisfy the Maxwell’s equations and ordinary Maxwell’s boundary conditions. The amplitudes of the fields decrease exponentially with increasing distance from the interface in both media. The electric field **E** has two components: *E*
_{
x
} along the propagation direction of the wave and *E*
_{
z
} perpendicular to the surface; the magnetic field **H** has only *y*-component.

*A*of the electric and magnetic fields in a surface wave, propagating along the

*x*-axis, has the following form:

*A*

_{0}is the amplitude,

*k*

_{p}is the propagation constant of the SPP,

*k*

_{1}>0 and

*k*

_{2}>0 are the damping factors of the surface electromagnetic wave in mediums 1 and 2, respectively, and

*t*is the time. The upper “ + ” sign refers to medium 1 where

*z*<0 and the lower “ −” sign refers to medium 2 where

*z*>0. The coefficients

*k*

_{1}and

*k*

_{2}are defined as

*H*of the magnetic field, it is possible to express the amplitudes of the electric fields as follows:

where *Z*
_{0}=(*μ*
_{0}/*ε*
_{0})^{1/2}.

### Appendix 2. Normal Pressure and Tangential Stress

*P*and

**S**of the surface force \(\pmb {{\mathcal {F}}}\) defined by Eq. 4 are readily found using the boundary conditions for the tangential components of

**E**and

**H**and normal components of

**D**and

**B**. Using the Maxwell-Lorentz stress tensor of Eq. 3, we obtain

In these equations, the the values of *P* and **S** are expressed through the electric field in medium 2. In the case of *μ*
_{1}=*μ*
_{2}, the surface force is independent of the magnetic field.

## Declarations

### Acknowledgements

The authors thank Saulius Juodkazis and M. G. Zubrilin for a bulk of experimental data on LIPSSs and discussions of the mechanisms of their formations.

**Open Access** This article is distributed under the terms of the Creative Commons Attribution 4.0 International License(http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

## Authors’ Affiliations

## References

- Bonse J, Rosenfeld A, Krüger J (2009) On the role of surface plasmon polaritons in the formation of laser-induced periodic surface structures upon irradiation of silicon by femtosecond laser pulses. J Appl Phys 106: 104910.View ArticleGoogle Scholar
- Bonse J, Krüger J, Höhm S, Rosenfeld A (2012) Femtosecond laser-induced periodic surface structure. J Laser Appl 24(4): 042006.View ArticleGoogle Scholar
- Bonse J, Höhm S, Rosenfeld A, Krüger J (2012) Sub-100-nm laser-induced periodic surface structures upon irradiation of titanium by Ti:sapphire femtosecond laser pulses in air. Appl Phys A 110: 547–551.View ArticleGoogle Scholar
- Vorobyev AY, Guo C (2008) Colorizing metals with femtosecond laser pulses. Appl Phys Lett 92: 041914.View ArticleGoogle Scholar
- Vorobyev AY, Guo C (2008) Femtosecond laser blackening of platinum. J Appl Phys 104: 053516.View ArticleGoogle Scholar
- Derrien TJ-Y, Itina TE, Torres R, Saints M (2013) Possible surface plasmon polariton excitation under femtosecond laser irradiation of silicon. J Appl Phys 114: 083104.View ArticleGoogle Scholar
- Mahmood AS, Venkatakrishnan K, Tan B (2013) 3-D aluminium nanostructure with microhole array synthesized by femtosecond laser radiation for enhanced light extinction. Nanoscale Res Lett 8: 477.View ArticleGoogle Scholar
- Mansuripur M, Zakharian AR, Lesuffleur A, Oh SH, Jones RJ, Lindquist NC, Im H, Kobyakov A, Moloney JV (2009) Plasmonic nano-structures for optical data storage. Opt Express 17(16): 14001–14014.View ArticleGoogle Scholar
- Birnbaum M (1965) Semiconductor surface damage produced by Ruby laser. J Appl Phys 36: 3688–3689.View ArticleGoogle Scholar
- Reif J, Varlamova O, Uhlig S, Varlamov S, Bestehorn M (2014) On the physics of self-organized nanostructure formation upon femtosecond laser ablation. Appl Phys A 117: 179–184.View ArticleGoogle Scholar
- Sipe JE, Young JF, Preston JS, van Driel HM (1983) Laser-induced periodic surface structure. I, Theory. Phys Rev B 27(2): 1141–1154.View ArticleGoogle Scholar
- Huang M, Zhao F, Cheng Y, Xu N, Xu Z (2009) Origin of laser-induced near-subwavelength ripples: interference between surface plasmon and incident laser. ACS Nano 3(12): 4062–4070.View ArticleGoogle Scholar
- Sakabe S, Hashida M, Tokita S, Namba S, Okamuro K (2009) Mechanism for self-formation of periodic grating structure on a metal surface by a femtosecond laser pulse. Phys Rev B 79: 033409.View ArticleGoogle Scholar
- Garrelie F, Colombier JP, Pigeon F, Tonchev S, Faure N, Bounhalli M, Reynaud S, Parriaux O (2011) Evidence of surface plasmon resonance in ultrafast laser-induced ripples. Opt Express 19(10): 9035–9043.View ArticleGoogle Scholar
- Tsibidis GD, Barberoglou M, Loukakos PA, Stratakis E, Fotakis C (2012) Dynamics of ripple formation on silicon surfaces by ultrashort laser pulses in subablation conditions. Phys Rev B 86: 115316.View ArticleGoogle Scholar
- Skolski JZP, Römer GRBE, Obona JV, Huis in’t Veld AJ, Hosson JTMD (2012) Laser-induced periodic surface structures: fingerprints of light localization. Phys Rev B 85: 075320.View ArticleGoogle Scholar
- Tsibidis GD, Stratakis E, Aifantis KE (2012) Thermoplastic deformation of silicon surfaces induced by ultrashort pulsed lasers in submelting conditions. J Appl Phys 111: 053502.View ArticleGoogle Scholar
- Kafka KRP, Austin DR, Li H, Yi A, Cheng J, Chowdhury EA (2015) Time-resolved measurement of single pulse femtosecond laser-induced periodic surface structure formation induced by a pre-fabricated surface groove. Opt Express 23(15): 19432–19441.View ArticleGoogle Scholar
- Bonch-Bruevich AM, Libenson MN, Makin VS, Trubaev VV, Vavilov SI (1992) Surface electromagnetic waves in optics. Opt Engin 31(4): 718–730.View ArticleGoogle Scholar
- Novotny J, Hecht B (2006) Principles of nano-optics. Cambridge University Press, New York.View ArticleGoogle Scholar
- Zakharian AR, Moloney JV, Mansuripur M (2007) Surface plasmon polaritons on metallic surfaces. Opt Express 15(1): 183–197.View ArticleGoogle Scholar
- Buividas R, Rosa L, Šliupas R, Kudrius T, Šlekys G, Datsyuk V, Juodkazis S (2011) Mechanism of fine ripple formation on surface of (semi)transparent materials via a half-wavelength cavity feedback. Nanotechnol 22: 055304.View ArticleGoogle Scholar
- Maxwell JC (1873) A treatise on electricity and magnetism. Vol. II. Clarendon Press, Oxford.Google Scholar
- Datsyuk VV, Pavlyniuk OR (2015) Maxwell stress on a small dielectric sphere in a dielectric. Phys Rev A 91(2): 023826.View ArticleGoogle Scholar
- Hebesberger T, Stüve HP, Vorhauer A, Wetscher F, Pippan R (2005) Structure of Cu deformed by high pressure torsion. Acta Mater 53: 393–402.View ArticleGoogle Scholar